• 검색 결과가 없습니다.

# Configurational force on a dynamic dislocation with localized oscillation

N/A
N/A
Protected

Share "Configurational force on a dynamic dislocation with localized oscillation "

Copied!
26
0
0

로드 중.... (전체 텍스트 보기)

전체 글

(1)

International Journal of Plasticity 136 (2021) 102814

Available online 21 July 2020

## Configurational force on a dynamic dislocation with localized oscillation

### Soon Kim, Hokun Kim, Sung Youb Kim

*

Department of Mechanical Engineering, Ulsan National Institute of Science and Technology, Ulsan, 44919, South Korea

A B S T R A C T

Upon employing the conservation theorem and continuum theory, the configurational force on a singularity, or a defect, is given by a path- independent integral called the J integral. According to the continuum elasticity theory, the J integral around a steadily moving dislocation is equal to the Peach–Koehler force acting on the dislocation and is independent of the integration path. However, using a discrete lattice dynamics method, we theoretically prove that the J integral is not path-independent in practice even under uniform motion. This is because of the generation of phonons during the dislocation motion. In general, phonons are generated upon localized oscillation of the dislocation, and they dissipate energy from the dislocation core; consequently, a drag force is produced. As the drag force disturbs the dislocation motion, the J integral around the moving dislocation is smaller than that around a stationary one, and its deviation from the stationary one corresponds to the drag force. In this study, we analytically derive the drag force for each oscillation mode by adopting dislocation–phonon coordinates. We classify the oscillation mode simply as symmetric or anti-symmetric after assuming the dislocation to be a localized defect having a finite core width. Consequently, the drag force is numerically calculated upon consideration of the discrete nature of the dislocation core. In particular, our study reveals that the anti-symmetric oscillation mode mainly contributes to the drag force in the limit of high dislocation velocity. Furthermore, we show that the resulting relation between the drag force and dislocation frequency can reproduce the dislocation velocity-stress curve. This work is expected to contribute to meso- and macro-scale plasticity when the material is loaded under extreme conditions or transient dislocation motion can be assumed.

1. Introduction

Macroscopic plastic deformation is an irreversible consequence of dislocation motion under external stress at the micro- and nano- scales. Therefore, numerous studies have been conducted to understand the plastic deformation in crystals, and accordingly, the collective dynamics of dislocation segments has been actively studied (Leung et al., 2015; Luscher et al., 2016, 2018). Especially, the more studies have been carried out to reflect the dislocation core effect on dislocation dynamics and plasticity in multi-scale frame- work (Amodeo et al., 2016; Liu et al., 2016; Jamond et al., 2016; Song et al., 2018; Swinburne et al., 2013; Zhang and Ngan, 2018).

Although it has been well proved that the dislocation core determines the dislocation mobility and cross-slip rate, there has been lack of effort to include the core effect in dislocation density-based model. To overcome this limit, it is necessary to quantitatively describe the short-range interactions and discrete description of the dislocation core. In particular, the dislocation core effect becomes more sig- nificant when the material is under dynamic or shock loadings (Gurrutxaga-Lerma et al., 2015; Shehadeh and Zbib, 2016; Cui et al., 2019) because the dislocation inertia term (, or effective mass), which is responsible to energy radiation from the accelerated dislo- cation, is not negligible. Recently, Gurrutxaga-Lerma et al. (2015) revealed that the dynamic yield stress is determined by the interference between elastic waves emitted from the dislocation core and elastic shockwave generated by rapid compression of the material.

* Corresponding author. EB5 801-6, 50 UNIST-gil, UNIST, Ulsan, 44919, South Korea.

Contents lists available at ScienceDirect

## International Journal of Plasticity

journal homepage: http://www.elsevier.com/locate/ijplas

https://doi.org/10.1016/j.ijplas.2020.102814

Received 30 March 2020; Received in revised form 17 June 2020; Accepted 18 June 2020

(2)

The dislocation core effect can be quantified by solving an equation of its motion. For this, the local driving force acting on the dislocation must be quantified. However, unlike the Newtonian force, the mass is not defined for defects (including the dislocation).

Instead, the net translational force on the defect can be quantified by defining a configurational force, or the J integral, given in the form of an integral (Eshelby, 1951; Rice, 1968). Without defining the defect mass, the J integral is directly obtained using the derivative of the Lagrangian of the system with respect to the translation coordinate of the defect. The J integral physically indicates the energy release rate for the defect translation, and the conservation theorem was used to prove that the J integral is independent of the integration path around a stationary defect (Noether, 1971). Therefore, the J integral has been widely used to predict the start and the direction of crack propagation (Kaczmarczyk et al., 2014; Ozenç et al., 2016; Guo and Li, 2017), effective fracture toughness of ¨ heterogeneous media (Hossain et al., 2014; Kuhn and Müller, 2016) and damage evolution inside the materials (Yuan and Li, 2019).

When the J integral is applied to the stationary dislocation, the J integral is equal to the Peach–Koehler (PK) force acting on it (Eshelby, 1956). The J integral has been widely applied to characterize various states of dislocations upon consideration of simple to complex cases (Lubarda and Markenscoff, 2007; Baxevanakis and Giannakopoulos, 2015; Ballarini and Royer-Carfagni, 2016; Lubarda, 2015;

Seo et al., 2018).

The J integral has been applied to dynamic defects, as well as stationary ones (Ni and Markenscoff, 2008; Arvanitakis et al., 2012;

Kuhn and Müller, 2016; Ozenç et al., 2016). Compared with the stationary ¨ J integral, the pseudo-momentum term additionally contributes to the dynamic J integral, but the path-independency is still maintained as long as the defect moves with a uniform velocity (Ni and Markenscoff, 2008). Consequently, the dynamic J integral is equal to the PK force acting on the dislocation, as in steady motion. Nevertheless, it is worthwhile to mention the drag force Fdrag acting opposite to the local driving force during the dislocation motion because it always exists as long as the dislocation glides. As the drag force is attributed to the rate of energy dissipation Q from ˙ the dislocation core, these terms can be related by Q˙= − Fdrag·v,where v is the dislocation velocity. Moreover, as the drag force influences the dislocation inertia through the equation of dislocation motion, the dislocation core width and its self-force change over time when the dislocation moves non-uniformly (Pellegrini, 2012). This implies that the drag may have influence on the configura- tional force on the moving dislocation.

The energy dissipation mechanisms caused by the drag force depend on external conditions. At a very low temperature (where the thermal effect is ignorable), the energy dissipation during the dislocation motion mainly originates from radiation damping. The ra- diation damping is generated by the nonlinearity-induced energy loss from long-to short-wavelength phonons (Kresse and Truski- novsky, 2003). By assuming the dislocation as an instability moving with uniform velocity in a discrete lattice, the rate of dissipation and the configurational force can be analytically derived as functions of the dislocation velocity (Wang and Abeyaratne, 2018). The discrete lattice model predicts that more phonons are emitted, and the emitted phonons have shorter wavelengths, as the dislocation velocity decreases. Furthermore, the emitted phonons are scattered by an anharmonic strain field around the dislocation core, which reduces the average stress around the dislocation core (Kim et al., 2016). If the thermal effect is considered, additional drag mech- anisms appear during the dislocation motion. In general, the influence of temperature on the drag mechanisms has been examined by normalizing it with respect to the Debye temperature, θD. (In most crystals, θD is approximately 200–400 K.) If the temperature is lower than approximately 0.1θD, phonon emission owing to the vibrating dislocation in the thermal field becomes the predominant source of energy dissipation (Ninomiya, 1974; Chen et al., 2017; Amrit et al., 2018). This is called flutter drag. In contrast to radiation damping, where only the excited waves whose phase velocities are equal to the dislocation velocity are radiated, arbitrary waves are emitted by the flutter drag. Furthermore, at a temperature higher than or equal to θD, phonon wind becomes the predominant drag mechanism (Al’Shitz and Indenbom, 1975; Blaschke, 2019a, 2019b; Blaschke et al., 2020a). In this case, anharmonic scattering of phonons by the moving dislocation imparts momentum to the latter in the opposite direction to the dislocation motion. In particular, when the dislocation velocity is comparable to the transverse sound wave speed, the aforementioned drag forces are amplified owing to the relativistic effect according to the continuum elasticity theory. Moreover, it has recently been proven that the relativistic effect can be alternatively explained by characterizing the dislocation as a spontaneous vibrating defect based on the discrete lattice dynamics (Kim et al., 2020).

In this study, we theoretically derive the J integral around a uniformly moving dislocation by considering the drag effect. We characterize the drag effect by assuming that the dislocation oscillates based on the lattice dynamics theory. Unlike the continuum theory, the lattice dynamics theory assumes the frequency spectrum of the system to be bounded. Therefore, the divergence problems that are presented in the field theory can be avoided. Depending on whether the frequencies newly generated by the dislocation deviate from the frequency band of the perfect lattice, the oscillation types are classified into two cases. First, if the dislocation frequency is above the maximum frequency of a perfect lattice, the oscillation amplitude is localized around the dislocation core; hence, it exponentially decays as the distance from the core increases. Thus, the dislocation core can be treated as an isolated defect (Lifshitz and Kosevich, 1966). This type of oscillation can be applied to a dynamic dislocation when the phonons are localized around the dislo- cation. In contrast, if the dislocation frequency exists within the frequency band of a perfect lattice, the waves are scattered rather than being localized. Thus, this type of oscillation can be applied when the phonon scattering is the dominant drag mechanism. Here, we only deal with the former type of oscillation, or the localized oscillation. And we express the drag force by using the dis- location–phonon coordinates rather than conventional atomic displacement coordinates. Subsequently, the dislocation oscillation is examined by solving a matrix eigenvalue problem, and finally, the contribution of each eigenmode to the drag force is revealed by considering the discrete nature of the dislocation core.

(3)

2. Continuum approach (revisited)

Before we discuss the main results of our study in the next section, we briefly introduce a derivation of the configurational force acting on a uniformly moving dislocation based on the continuum theory. This derivation was undertaken by Stroh (1962). We summarize it here to show that the J integral calculated for a static dislocation can still be identically applied to a moving dislocation, unless it accelerates. The detailed derivation is presented in Appendices A and B based on Stroh’s (1962) work.

Imagine a system consisting of two separated regions I and II as in Fig. 1. In region I, a dislocation loop, which is denoted as D, is inserted and it is surrounded by a surface Σi. Thus, Σi has a tube shape whose radius is a. Assume that there are other singularities or stress sources, denoted as S, in region II, which are surrounded by the inner and outer surfaces, Σi and Σo, respectively. Thus, we can express the total Lagrangian of the system, L, as

L=LD+LS+LDS (1)

where LD and LS are the Lagrangians of D and S, respectively, and LDS is the Lagrangian caused by the interaction between them. As the dislocation moves, the distance between D and S changes, which will cause a change in LDS. If ξ specifies the position of the dislocation, the configurational force acting on the dislocation along the ξ direction, Fξ, is defined as

t2

t1

Fξδξ dt=δ

t2

t1

LDSdt. (2)

According to Appendix A, LDS is derived as LDS=TDSUDS= − bi

C

σSijdSj +

І+ІІ

ρd dt

(uDivSi)

d3x, (3)

where σS and vS are the stress and material velocity caused by S, respectively, and uD is the displacement caused by D. Here, ρ is the density of the system. The configurational force can be derived by using Eq. (2) and Eq. (3). Assume that the dislocation loop, D, moves by an infinitesimal distance, δξ, as shown in Fig. 2. Then, according to Appendix B, a variation of Eq. (3) can be derived as

δLDS=δLDS1 +δLDS2 =bi

σSijεjkldskδξl+

І+ІІ

ρd dt

(δuDivSi)

d3x (4)

where δLDS1 =bi

σSijεjkldskδξl, (5)

δLDS2 =

І+ІІ

ρd dt

(δuDivSi)

d3x. (6)

Then, the force acting on D, to which δLDS1 contributes, is derived as Eq. (7), which is the PK force, from Eq. (2).

F1ξ=biσSijεjkltk, (7)

where tk is the unit dislocation line vector. Furthermore, δLDS2 is derived as

Fig. 1.(a) System including a dislocation loop D in region I and other singularities S in region II. (b) Enlarged view of the dislocation loop D. Here, the dislocation is surrounded by a cylindrical tube whose radius is a. In both (a) and (b), the shaded region represents the area slipped by the dislocation loop.

(4)

δLDS2 =

Σi

ρδuDivSiξ˙jdSj +

І

ρvSid dt

(δuDi)

d3x. (8)

Here, δLDS2 depends on the material velocity, vS, or the velocity of the observer. In this study, the frame of the observer does not move so that vS =0. Therefore, the configurational force acting on the dynamic dislocation is calculated by using Eq. (7), which is equal to the PK force defined for a stationary dislocation. However, even if the frame of the observer moves, the equivalence is still satisfied, unless the frame accelerates. This is because we can make δuD arbitrarily small inside region I, according to the continuity assumption, by suitably restricting δξ. Consequently, it is possible to make the contribution of δLDS2 arbitrarily small compared with that of δLDS1 to the configurational force. In fact, Eq. (8) is responsible for a force called the Lorentz force, but it was proved that this force does not influence the dislocation glide (Lothe, 1961; Stroh, 1962; Kosevich, 1965).

3. Discrete lattice approach 3.1. Coordinate transformation

In mechanics, the Lagrangian of a system is generally described in terms of the displacements of constituent atoms. However, as we intend to describe the interaction between the strain field around the dislocation and the phonons directly, we change the conventional displacement coordinate system to a dislocation–phonon coordinate system by adopting the dislocation coordinate, which was first suggested by Ninomiya (1972). First, we introduce the coordinate transformation based on Ninomiya’s (1972) work. Subsequently, we define the J integral around a dynamic dislocation in the transformed coordinate system.

We simplify the system into a one-dimensional chain consisting of N atoms. Thus, the system has N degrees of freedom (DOFs).

However, as a single dislocation is inserted inside the system, the DOFs of the system are reduced to N− 1,as 1-DOF is assigned to Fig. 2. Motion of the dislocation loop.

Fig. 3.Simple description of the N-dimensional potential energy surface as a function of atomic displacements. If there is no defect, the system is located at a valley “G.” In contrast, if the dislocation is inserted, then the system is located at a valley “L.”

(5)

describe the strain field of the dislocation. If we plot the energy of the system as a function of N dimensional abscissas, {u1,u2,,uN}, where un corresponds to the displacement of the n-th atom, the energy surface is presented as shown in Fig. 3. The figure shows two valleys. The global minimum state (state G) corresponds to the system with no defects, whereas the local minimum state (state L) corresponds to the system where the dislocation is inserted. As the dislocation glides, the state of the system will move along the local minimum valley on theN-dimensional energy surface with the change in the displacement of each atom over time. Accordingly, we can define the dislocation coordinate, ξ, as a collective variable expressed in terms of {udis1 ,udis2,,udisN}, where udisn is the displacement of the n-th atom required to accommodate the dislocation. Physically, ξ represents the position of the dislocation. If 1-DOF is assigned to ξ, then N− 1 DOFs remain. These remaining DOFs are orthogonal to ξ, and hence, they induce the climbing of the sides of the local minimum valley in Fig. 3. Physically, these N− 1 variables correspond to the phonons that disturb the dislocation glide along the local energy minimum valley, and hereafter, we define them as phonon coordinates.

If the dislocation is in a static equilibrium state, the displacement field around it, ws(xξ), can be described as shown in Fig. 4(a). If it is defined by using λ(1)(xξ),

ws(xξ) =

ξ

λ(1)(xξ’), (9)

then λ(1)(xξ) =dws/dξ is satisfied and it becomes a localized function around ξ as described in Fig. 4(b). Here, λ(1)(xξ)is normalized as

n

(λ(1)(nbξ))2=1. (10)

Moreover, ws(xξ)should satisfy Eq. (11) as a boundary condition.

ξ→∞limws(xξ) =b, (11)

where b is the Burgers vector. Hereafter, we use the alternate expression λ(1)n (ξ) ≡λ(1)(nbξ)and wn(ξ) ≡ws(nbξ)for convenience.

From the shape of λ(1)n (ξ)in Fig. 4(b), it can be inferred that λ(1)n (ξ)physically indicates the compactness of the dislocation core.

Moreover, if we define additional variables, λ(nj)(ξ)for j=1,2,,N and express the atomic displacement un by using {λ(n1)(n2),, λ(N)n }, Eq. (12) can be derived.

un=wn(ξ) +∑N

v=2

τvλ(v)n (ξ). (12)

Here, as λ(1)n (2)n ,(N)n should be orthogonal to each other, Eq. (13) follows.

n

λ(nμ)(ξ)λ(v)n (ξ) =δμv (μ,v=1,2,,N), (13)

where δμv is the Kronecker delta. As the dislocation glides, phonons are generated, and they cause an additional atomic displacement, which makes the system deviate from the static equilibrium state. The contribution of the phonons to the displacement is reflected by the second term on the right-hand side (RHS) of Eq. (12). By using Eq. (12), the Lagrangian can be expressed in terms of the new coordinates {ξ,τ2,N}. However, it is not practical because λ(2)n ,(N)n are not known and the constraint, Eq. (13), complicates the calculation.

To avoid these drawbacks, Ninomiya (1972) suggested a method in which a basis set is changed by adding a single redundant variable, τ1, to the system. Consequently, the total number of variables becomes N+1 and the DOF of the system becomes N.

Physically, the addition of the variable corresponds to the addition of an isolated free oscillator to the dislocated system, Lsys. The

Fig. 4.(a) Dislocation displacement field under a static equilibrium state. (b) Compactness function of the dislocation core. Here, λ(1)(xξ) =dws/ and λ(1)is assumed as a Gaussian distribution function whose mean is ξ and standard deviation is σD. We assumed that the dislocation core width is 2σD in this study.

(6)

2m˙τ21− 1

221τ21, (14)

where m is the atomic mass and ω1 is the frequency of the added oscillator. And if we define new variables as υn=∑N

v=1

τvλ(v)n (ξ),

τv=∑N

n=1

υnλ(v)n (ξ),

(15)

we can express un and τ1, respectively, in terms of these new variables as

un=wn(ξ) +∑N

v=2

τvλ(v)n (ξ) =wn(ξ) +υnτ1λ(1)n (ξ) =wn(ξ) +υn− (∑N

m=1

υmλ(1)m(ξ) )

λ(1)n (ξ), (16-1)

τ1=∑N

n=1

υnλ(1)n (ξ). (16-2)

In Eq. (16–1) and Eq. (16–2), as λ(n2),(n N)are not required, whereas only λ(n1), which is explicitly known, is used, the coordinate transformation from {u1,u2,,uN1}to {ξ,υ12,N}can be conveniently undertaken. Furthermore, the orthogonality constraint is automatically reflected to relate υn and τv in Eq. (15), and no constraint is necessary. Consequently, the transformed coordinate system consists of the dislocation coordinate, ξ, and N phonon coordinates, υ12,N.

3.2. J integral in dislocationphonon coordinate system

The J integral can be derived by using the transformed coordinate system, {ξ,υ12,N}. As the J integral physically indicates a translational configurational force per unit length of the dislocation, it can be defined by using the dislocation coordinate as

J= − 1 l

Lsys

ξ = − 1 l

(∂Tsys

ξ − 1 l

Usys

ξ )

, (17)

where l is the length of the dislocation, and Tsys and Usys are the kinetic and potential energies of the system, respectively. Here, Tsys and Usys are expressed, respectively, as

Tsys=1 2mN

n=1

u˙2n, (18-1)

Usys=1 2γN

n=2

(unun1)2+

N

n=1

V(un), (18-2)

where γ is the spring constant and V is the substrate potential. The kinetic term in Eq. (17) becomes zero and this is proved in Appendix C. Similarly, the potential term in Eq. (17) is expressed as follows:

Usys

ξ =∑N

n=1

Usys

un

un

ξ +∂Usys

τ1

τ1

ξ, (19)

From Eq. (16–1),

un

ξ=dwn

− [

(1)n

N

m=1

λ(1)mυm+λ(1)nN

m=1

(1)m dξυm

]

(20)

is derived. By using ∂Usys/τ1 =0, and substituting Eq. (19) andEq. (20) into Eq. (17), the J integral is derived as

J=1 l

N

n=1

Usys

un

dwn

− 1 l

N

n=1

Usys

un

( n

N

m=1

λmυm+λn

N

m=1

m

dξυm

)

, (21)

Here, λ(1)n was replaced by λn for convenience.

Given that λn(ξ)is a localized function around ξ, we assume that it is a Gaussian distribution function as defined in Eq. (22).

λn(ξ) =λ(r;ξ) = b σD

̅̅̅̅̅

2π

e

(rξ)2 2σ2

D, (22)

(7)

where r=nb and σD is the standard deviation of the distribution function and is a parameter characterizing the size of the dislocation core. In other words, we describe the dislocation core as a diffusive zone, whose width is approximately 2σD. Note that Eq. (22) also satisfies the boundary condition, Eq. (11). As ∂Usys/un = (τapp+τdis)lb, where τdis is the dislocation stress field and dwn/dξ = λn, the first term on the RHS of Eq. (21) in the continuum limit becomes

J1=1 l

n

Usys

un

dwn

≈1 lb

Usys

u dw dr=

(τapp+τdis

)λ(r;ξ)dr. (23)

According to the linear elasticity theory, as τdis∼1/r, τdis =C/r, where C is a constant, is substituted into Eq. (23). Moreover, we assume that the dislocation is at the origin, and hence, ξ =0. Subsequently, Eq. (23) results in Eq. (24). Here, the τdis term disappears because it is an odd function.

J1b σD

̅̅̅̅̅

2π

( τapp+C

r )

e

r2 2σ2

Ddr=τappb. (24)

Therefore, the first term of Eq. (21) is equal to the PK force, FPK, defined in the continuum theory. Unlike the first term, the second term of Eq. (21) includes the phonon coordinates, υn. Accordingly, it can be inferred that the second term in Eq. (21) is generated because of the interaction between the dislocation and the phonons. This term is the main interest of this study, and we define it as Fdrag. Consequently, the J integral around the dynamic dislocation that interacts with the phonons consists of two separate terms, i.e.,

J=FPK+Fdrag, (25)

where

FPK=τappb, (26-1)

Fdrag= − 1 l

N

n=1

Usys

un

( n

N

m=1

λmυm+λn

N

m=1

m

dξυm

)

. (26-2)

As an extreme example, if the dislocation does not move, phonons are not generated from the dislocation core. Consequently, υn will be zero for every atom; hence, the J integral will be equal to FPK, as in the continuum theory. Thus, Eq. (25) reconfirms that the phonons are responsible for dragging the moving defect (Slepyan, 2001; Kresse and Truskinovsky, 2003; Kim et al., 2016).

To simplify Eq. (26–2), C in τdis should be analytically obtained using the following process. As it was proved that Eq. (23) is equal to the PK force in the continuum limit, the M integral can be defined in the discrete lattice similarly. Based on the definition of the M integral in the continuum theory (Budiansky and Rice, 1973; Agiasofitou and Lazar, 2017), M1 with no drag effect can be simply derived in the continuum limit as

M1

r( τapp+τdis

)λ(r;ξ)dr=

r (

τapp+C r )

λ(r;ξ)dr=Cb. (27)

Here, the τapp term has disappeared, as (r)is an odd function. According to the continuum theory, M1=Gb2/4π in a two- dimensional system. Here, G is shear modulus. Therefore, C=Gb/4π is obtained. Then, as we replace the discrete sums with in- tegrals from r= − R to r=R in Eq. (26–2), Fdrag becomes

Fdrag=1 l

N

n=1

Usys

un

( n

N

m=1

λmυm+λn

N

m=1

m

dξυm

)

=1 l

[(∑

n

Usys

un

n

)(∑N

m=1

λmυm

) +

(∑

n

Usys

un

λn

)(∑N

m=1

m

dξυm

)]

=

R

R

( τapp+Gb

4πr )

dξdr·1 b

R

R

λ(r)υ(r)dr

⎦+

R

R

( τapp+Gb

4πr )

λ(r)dr·1 b

R

R

dξυ(r)dr

.

(28)

If we substitute dλ/dξ= [b(rξ)/(σ3D̅̅̅̅̅̅2π)]exp(− (rξ)2/2σ2D)with ξ=0 into Eq. (28) and delete the odd terms, Eq. (28) is simplified to

Fdrag= − b σ3D̅̅̅̅̅2π

⎢⎣Gb 4π

R

R

υ(r)e

r2 2σ2

Ddr+τapp

R

R

(r)e

r2 2σ2

Ddr

⎥⎦. (29)

If we restore the discreteness, then the drag force can also be represented as

(8)

Fdrag= − b σ3D̅̅̅̅̅2π

⎢⎢

Gb2

4π

R/b

j=−R/b

υ(j)e

(jb)2 2σ2

D+τappb2R/b

j=−R/b

(j)e

(jb)2 2σ2

D

⎥⎥

. (30)

This will be used for the numerical calculation of the drag force in Section 4. Two points can be inferred from the closed form of Eq.

(29). First, the phonons contribute to the drag force in two ways by interacting with the strain fields caused by the dislocation and external stress. Among them, the interactions near the dislocation core are mainly responsible for the drag force because the expo- nential terms in Eq. (29) decay rapidly, as the distance from the center of the core increases. Second, the drag force depends on the integration size, R. In other words, the existence of the drag force makes the J integral path-dependent.

3.3. Phonon coordinates and eigenmodes

According to Eq. (29) (or Eq. (30)), the drag force can be calculated only after the phonon coordinates, υ(r)(orυ(j)), are deter- mined. In general, a wave can be analyzed by decomposing it into elementary normal modes (called eigenmodes) depending on the DOF of the system. Similarly, the phonon coordinate, or the oscillation displacement, can be decomposed into a finite number of eigen- modes, where all the atoms oscillate with the same frequency. Given that the phonon coordinate is expressed by a linear combination of the eigenmodes, determining the contribution of each eigenmode to the drag force is our primary objective. In this section, we derive the phonon coordinate of each eigenmode by simplifying the dislocation as a localized defect based on the method developed by Montroll and Potts (1955) and investigate the influence of the phonon coordinate on the drag force. The authors analyzed the oscillation of a point defect by solving an eigenvalue problem. However, as the dislocation core width is an important factor to determine the drag force in this study, we extended their method to a defect whose core has a finite width.

In a one-dimensional atomic chain with a defect, the displacement of the j-th atom can be obtained by solving Eq. (31).

m¨xj+γ[

xj+1− 2xj+xj1

]=Dxj, (31)

where m is the atomic mass, γ is the spring constant, and D is an operator characterizing the defect or dislocation. Under the plane wave assumption, xj =υ(j)exp( − iωt), Eq. (31) is modified to

(j) =2υ(j) +γ[υ(j+1) − 2υ(j) +υ(j− 1)], (32)

where L= − D. Furthermore, we can express the RHS of Eq. (32) in a matrix form by defining w(i)(j)as (j) =2υ(j) +γ[υ(j+1) − 2υ(j) +υ(j− 1)] ≡∑

k

w(k)(k+j)υ(k+j). (33)

Before solving Eq. (33), it is convenient to define a function g(j)that satisfies

Lg(xs) =γδ(xs). (34)

Here, g(j)is the (lattice) Green’s function. If we multiply an arbitrary function, f(s), to both sides of Eq. (34) and integrate over S, then Eq. (35) is derived.

f(x) =1 γ

Lg(xs)f(s)ds. (35)

Therefore, to solve the equation (j) =f(j), it can be alternatively expressed by (j) =1

γ

Lg(js)f(j)ds=L (1

γ

g(js)f(j)ds )

. (36)

Thus, we can obtain υ(j)as υ(j) =1

γ

g(js)f(j)ds. (37)

From Eq. (33) and Eq. (37), υ(j) =γ1

m

k

g(jm)w(k)(k+m)υ(k+m). (38)

If k+m is replaced by l, then υ(j)is derived as υ(j) =γ1

m

l

g(j+kl)w(k)(l)υ(l). (39)

To define g(j), let us express it in terms of the Fourier transform as

(9)

g(j) =1 2π

G(φ)eiφjdφ. (40)

By substituting Eq. (40) into Eq. (32) and using Eq. (34), Eq. (41) is derived.

γδ(j) =1 2π

G(φ)[

2+2γ(cosφ− 1)]

eiφjdφ. (41)

As δ(j) = (1/2π)

exp( − iϕj)dϕ,

G(φ) = γ

2+2γ(cosφ− 1). (42)

If we substitute Eq. (42) into Eq. (40) and confine the integration range to the first Brillouin zone, the Green’s function is derived as

g(j) =γ π

π

0

cosφj

2+2γ(cosφ− 1)dφ. (43)

Depending on the frequency, ω, the integrand of Eq. (43) either has poles or does not. In a perfect lattice system without any defects, the maximum reachable frequency, ωL, is 2 ̅̅̅̅̅̅̅̅̅

γ/m

√ . If ωωL, the integrand has poles, but if ω>ωL, it does not have poles. In this study, we only consider the latter. In this case, the frequency bands newly generated by embedding the dislocation are localized around the atoms of the dislocation core (Kim et al., 2020). Therefore, υ(j)→0 as j→±∞. In general, this occurs when the drag force is governed by the inertial oscillation resulting from the extremely high speed of the dislocation (Gurrutxaga-Lerma, 2016; Peng et al., 2019). If we define fω/ωL≡cosh(z/2)and assume that f>1, then Eq. (43) is modified to

g(j) =1 2π

π

0

cosφj

cosφ+coshzdφ (44)

As cosh(z)>1, the integrand does not have poles. According to Montroll and Potts (1955), Eq. (44) finally yields g(j) =( − 1)j

2sinhze− |j|z (45)

As the dislocation core is localized, it is reasonable to assume that the index l in Eq. (39) only includes atoms in the core rather than in the entire system. Thus, Eq. (39) can be expressed in a matrix form as

υ=. (46)

If we define an eigenvector and eigenvalue of T in mode μ as Ψμ and βμ, respectively, then

μ=βμΨμ (47)

is satisfied. Moreover, if we express υ in terms of the basis Ψμ as υ=∑

μυμΨμ, then Eq. (46) is modified to ∑

μυμ(1− βμ)Ψμ = 0. For Eq.

(46) to have solutions, βμ=1 must be satisfied for all eigenmodes μ.

As shown in Fig. 5, we assume that the center of the core is at the origin and 2σG+1 atoms are geometrically defined as the dislocation core. The core atoms are connected by a spring whose constant is γ’ but the others are connected by γ. If we define an atomic

Fig. 5.Discrete lattice model for dislocation oscillation. All the atoms are attached to substrate potential, V. As the dislocation glides to the right, the atoms moves to phase 2, or neighboring valley, from phase 1. The shaded atoms represent the dislocation core whose radius is σGb, and they are connected by an elastic spring whose stiffness is γ’. But atoms outside of the core region are connected by the spring whose stiffness is γ.

(10)

mass as m, the equations of motion are given by

(i) (j) = (γγ’)[υ(j+1) − 2υ(j) +υ(j− 1)] ( − σGjσG) (ii) (σG+1) = (γ’− γ)[υ(σG+1) − υ(σG)]

(iii) ( − σG− 1) = (γγ’)[υ( − σG) − υ( − σG− 1)]

(48) By comparing Eq. (48) with Eq. (33), the following relations can be obtained:

(i) w(−1)(j− 1) =w(1)(j+1) =γγ, w(0)(j) = − 2(γγ’) ( − σGj≤ − σG) (ii) w(−1)(σG) =γγ, w(0)(σG+1) =γ’− γ

(iii) w(−1)( − σG− 1) =γ’− γ, w(0)( − σG) =γγ

(49)

By substituting the relations Eq. (49) into Eq. (39), Eq. (50) is derived.

υ(j) =γ1[(γγ’)g(j+σG) + (γγ’)g(j+σG+1)]υ( − σG− 1) +γ1[(γγ’)g(j+σG− 1) − 2(γγ’)g(j+σG) + (γγ’)g(j+σG+1)]υ( − σG) +⋯γ1[(γγ’)g(jσG− 1) − 2(γγ’)g(jσG) + (γγ’)g(jσG+1)]υ(σG)

+γ1[(γ’− γ)g(jσG− 1) + (γγ’)g(jσG)]υ(σG+1).

(50)

If we define Pγ, then Eq. (50) is simplified to υ(j) = (1− P)[g(j+σG) − g(j+σG+1)]υ( − σG− 1)

+(1− P)[g(jσG) − g(jσG− 1)]υ(σG+1) + ∑σG

n=−σG

[(1− P){g(jn− 1) +g(jn+1)} − 2(1− P)g(jn)]υ(n)

(51)

Here, the Σ term that represents the displacement inside the core should be carefully considered because of the characteristic of the Green’s function. By substituting the Green’s function into Eq. (32),

Lg(j) =2g(j) +γ[g(j+1) − 2g(j) +g(j− 1)]

=γ[

4f2g(j) + {g(j+1) − 2g(j) +g(j− 1)}]

. (52)

is derived. Moreover, by using Eq. (34),

g(j+1) − 2g(j) +g(j− 1) = − 4f2g(j) (53)

is satisfied for j∕=0 and

4f2g(0) +g(1) − 2g(0) +g( − 1) =1 (54)

is satisfied for j =0. Then, the Σ term in Eq. (51) follows

(1− P){g(jn− 1) +g(jn+1)} − 2(1− P)g(jn) =4f2(P− 1)g(jn) (55-1) if j∕=n and

(1− P){g(jn− 1) +g(jn+1)} − 2(1− P)g(jn) = (1− P)(

− 4f2g(0) +1)

(55-2) when j =n. Thus, Eq. (51) becomes

υ(j) = (1− P)[g(j+σG) − g(j+σG+1)]υ( − σG− 1) +(1− P)[g(jσG) − g(jσG− 1)]υ(σG+1) − 4f2(1− P) ∑σG

m=−σG

g(jm)υ(m) (56-1)

if j<σG or j>σG and it represents the phonon coordinate outside the core. Then, Eq. (51) becomes υ(j) = (1− P)[g(j+σG) − g(j+σG+1)]υ( − σG− 1) + (1− P)[g(jσG) − g(jσG− 1)]

υ(σG+1) − 4f2(1− P) ∑σG

m=−σG (m=j)

g(jm)υ(m) + (1− P)[

− 4f2g(0) +1]

υ(j) (56-2)

when − σGjσG,and thus, it represents the phonon coordinate inside the core. Now, Eq. (56–1) and Eq. (56–2) can be expressed by the matrix equation in Eq. (57) by using the relation g( − j) =g(j).

참조

관련 문서

Androgen deprivation therapy is an important therapeutic option for prostate cancer; however, a substantial proportion of prostate cancers progress into